Concrete, usually Portland cement concrete, is a composite material composed of fine and coarse aggregate bonded together with a fluid cement (cement paste) that hardens over time—most frequently a lime-based cement binder, such as Portland cement, but sometimes with other hydraulic cements, such as a calcium aluminate cement. It is distinguished from other, non-cementitious types of concrete all binding some form of aggregate together, including asphalt concrete with a bitumen binder, which is frequently used for road surfaces, and polymer concretes that use polymers as a binder.
When aggregate is mixed together with dry Portland cement and water, the mixture forms a fluid slurry that is easily poured and molded into shape. The cement reacts chemically with the water and other ingredients to form a hard matrix that binds the materials together into a durable stone-like material that has many uses. Often, additives (such as pozzolans or superplasticizers) are included in the mixture to improve the physical properties of the wet mix or the finished material. Most concrete is poured with reinforcing materials (such as rebar) embedded to provide tensile strength, yielding reinforced concrete.
Famous concrete structures include the Hoover Dam, the Panama Canal and the Roman Pantheon. The earliest large-scale users of concrete technology were the ancient Romans, and concrete was widely used in the Roman Empire. The Colosseum in Rome was built largely of concrete, and the concrete dome of the Pantheon is the world's largest unreinforced concrete dome. Today, large concrete structures (for example, dams and multi-story car parks) are usually made with reinforced concrete.
After the Roman Empire collapsed, use of concrete became rare until the technology was redeveloped in the mid-18th century. Worldwide, concrete has overtaken steel in tonnage of material used.
The word concrete comes from the Latin word "concretus" (meaning compact or condensed), the perfect passive participle of "concrescere", from "con-" (together) and "crescere" (to grow).
Small-scale production of concrete-like materials dates to 6500 BC, pioneered by the Nabatean traders who occupied and controlled a series of oases and developed a small empire in the regions of southern Syria and northern Jordan. They discovered the advantages of hydraulic lime, with some self-cementing properties, by 700 BC. They built kilns to supply mortar for the construction of rubble-wall houses, concrete floors, and underground waterproof cisterns. They kept the cisterns secret as these enabled the Nabataeans to thrive in the desert. Some of these structures survive to this day.
German archaeologist Heinrich Schliemann found concrete floors, which were made of lime and pebbles, in the royal palace of Tiryns, Greece, which dates roughly to 1400–1200 BC. Lime mortars were used in Greece, Crete, and Cyprus in 800 BC. The Assyrian Jerwan Aqueduct (688 BC) made use of waterproof concrete. Concrete was used for construction in many ancient structures.
The Romans used concrete extensively from 300 BC to 476 AD, a span of more than seven hundred years. During the Roman Empire, Roman concrete (or opus caementicium) was made from quicklime, pozzolana and an aggregate of pumice. Its widespread use in many Roman structures, a key event in the history of architecture termed the Roman Architectural Revolution, freed Roman construction from the restrictions of stone and brick materials. It enabled revolutionary new designs in terms of both structural complexity and dimension.
Concrete, as the Romans knew it, was a new and revolutionary material. Laid in the shape of arches, vaults and domes, it quickly hardened into a rigid mass, free from many of the internal thrusts and strains that troubled the builders of similar structures in stone or brick.
Modern tests show that opus caementicium had as much compressive strength as modern Portland-cement concrete (ca. 200 kg/cm2 [20 MPa; 2,800 psi]). However, due to the absence of reinforcement, its tensile strength was far lower than modern reinforced concrete, and its mode of application was also different:
Modern structural concrete differs from Roman concrete in two important details. First, its mix consistency is fluid and homogeneous, allowing it to be poured into forms rather than requiring hand-layering together with the placement of aggregate, which, in Roman practice, often consisted of rubble. Second, integral reinforcing steel gives modern concrete assemblies great strength in tension, whereas Roman concrete could depend only upon the strength of the concrete bonding to resist tension.
The long-term durability of Roman concrete structures has been found to be due to its use of pyroclastic (volcanic) rock and ash, whereby crystallization of strätlingite and the coalescence of calcium–aluminum-silicate–hydrate cementing binder helped give the concrete a greater degree of fracture resistance even in seismically active environments. Roman concrete is significantly more resistant to erosion by seawater than modern concrete; it used pyroclastic materials which react with seawater to form Al-tobermorite crystals over time.
The widespread use of concrete in many Roman structures ensured that many survive to the present day. The Baths of Caracalla in Rome are just one example. Many Roman aqueducts and bridges, such as the magnificent Pont du Gard in southern France, have masonry cladding on a concrete core, as does the dome of the Pantheon.
After the Roman Empire, the use of burned lime and pozzolana was greatly reduced until the technique was all but forgotten between 500 and the 14th century. From the 14th century to the mid-18th century, the use of cement gradually returned. The Canal du Midi was built using concrete in 1670.
Perhaps the greatest step forward in the modern use of concrete was Smeaton's Tower, built by British engineer John Smeaton in Devon, England, between 1756 and 1759. This third Eddystone Lighthouse pioneered the use of hydraulic lime in concrete, using pebbles and powdered brick as aggregate.
A method for producing Portland cement was developed in England and patented by Joseph Aspdin in 1824. Aspdin chose the name for its similarity to Portland stone, which was quarried on the Isle of Portland in Dorset, England. His son William continued developments into the 1840s, earning him recognition for the development of "modern" Portland cement.
Reinforced concrete was invented in 1849 by Joseph Monier. and the first house was built by François Coignet in 1853. The first concrete reinforced bridge was designed and built by Joseph Monier in 1875.
Concrete is a composite material, comprising a matrix of aggregate (typically a rocky material) and a binder (typically Portland cement or asphalt), which holds the matrix together. Many types of concrete are available, determined by the formulations of binders and the types of aggregate used to suit the application for the material. These variables determine strength, density, as well as chemical and thermal resistance of the finished product.
A cement, most commonly Portland cement, is the most prevalent kind of concrete binder. For cementitious binders, water is mixed with the dry powder and aggregate, which produces a semi-liquid slurry that can be shaped, typically by pouring it into a form. The concrete solidifies and hardens through a chemical process called hydration. The water reacts with the cement, which bonds the other components together, creating a robust stone-like material. Other cementitious materials, such as fly ash and slag cement, are sometimes added as mineral admixtures – either pre-blended with the cement or directly as a concrete component – and become a part of the binder for the aggregate. Chemical admixtures are added to achieve varied properties. These ingredients may accelerate or slow down the rate at which the concrete hardens, and impart many other useful properties including increased tensile strength, entrainment of air and water resistance.
Mineral admixtures have become more popular over recent decades. The use of recycled materials as concrete ingredients has been gaining popularity because of increasingly stringent environmental legislation, and the discovery that such materials often have complementary and valuable properties. The most conspicuous of these are fly ash, a by-product of coal-fired power plants; ground granulated blast furnace slag, a byproduct of steelmaking; and silica fume, a byproduct of industrial electric arc furnaces. The use of these materials in concrete reduces the amount of resources required, as the mineral admixtures act as a partial cement replacement. This displaces some cement production, an energetically expensive and environmentally problematic process, while reducing the amount of industrial waste that must be disposed of. Mineral admixtures can be pre-blended with the cement during its production for sale and use as a blended cement, or mixed directly with other components when the concrete is produced.
Structures employing Portland cement concrete usually include steel reinforcement. Such concrete can be formulated with high compressive strength, but always has lower tensile strength. Therefore, it is usually reinforced with materials that are strong in tension, typically steel rebar.
The mix design depends on the type of structure being built, how the concrete is mixed and delivered, and how it is placed to form the structure.
Portland cement is the most common type of cement in general usage. It is a basic ingredient of concrete, mortar and many plasters. British masonry worker Joseph Aspdin patented Portland cement in 1824. It was named because of the similarity of its color to Portland limestone, quarried from the English Isle of Portland and used extensively in London architecture. It consists of a mixture of calcium silicates (alite, belite), aluminates and ferrites – compounds which combine calcium, silicon, aluminum and iron in forms which will react with water. Portland cement and similar materials are made by heating limestone (a source of calcium) with clay or shale (a source of silicon, aluminum and iron) and grinding this product (called clinker) with a source of sulfate (most commonly gypsum).
In modern cement kilns many advanced features are used to lower the fuel consumption per ton of clinker produced. Cement kilns are extremely large, complex, and inherently dusty industrial installations, and have emissions which must be controlled. Of the various ingredients used to produce a given quantity of concrete, the cement is the most energetically expensive. Even complex and efficient kilns require 3.3 to 3.6 gigajoules of energy to produce a ton of clinker and then grind it into cement. Many kilns can be fueled with difficult-to-dispose-of wastes, the most common being used tires. The extremely high temperatures and long periods of time at those temperatures allows cement kilns to efficiently and completely burn even difficult-to-use fuels.
As stated by Abrams' law, a lower water-to-cement ratio yields a stronger, more durable concrete, whereas more water gives a freer-flowing concrete with a higher slump. Impure water used to make concrete can cause problems when setting or in causing premature failure of the structure.
Hydration involves many different reactions, often occurring at the same time. As the reactions proceed, the products of the cement hydration process gradually bond together the individual sand and gravel particles and other components of the concrete to form a solid mass.
- Cement chemist notation: C3S + H → C-S-H + CH
- Standard notation: Ca3SiO5 + H2O → (CaO)·(SiO2)·(H2O)(gel) + Ca(OH)2
- Balanced: 2Ca3SiO5 + 7H2O → 3(CaO)·2(SiO2)·4(H2O)(gel) + 3Ca(OH)2 (approximately; the exact ratios of the CaO, SiO2 and H2O in C-S-H can vary)
Fine and coarse aggregates make up the bulk of a concrete mixture. Sand, natural gravel, and crushed stone are used mainly for this purpose. Recycled aggregates (from construction, demolition, and excavation waste) are increasingly used as partial replacements for natural aggregates, while a number of manufactured aggregates, including air-cooled blast furnace slag and bottom ash are also permitted.
The size distribution of the aggregate determines how much binder is required. Aggregate with a very even size distribution has the biggest gaps whereas adding aggregate with smaller particles tends to fill these gaps. The binder must fill the gaps between the aggregate as well as paste the surfaces of the aggregate together, and is typically the most expensive component. Thus, variation in sizes of the aggregate reduces the cost of concrete. The aggregate is nearly always stronger than the binder, so its use does not negatively affect the strength of the concrete.
Redistribution of aggregates after compaction often creates inhomogeneity due to the influence of vibration. This can lead to strength gradients.
Decorative stones such as quartzite, small river stones or crushed glass are sometimes added to the surface of concrete for a decorative "exposed aggregate" finish, popular among landscape designers.
In addition to being decorative, exposed aggregate may add robustness to a concrete.
Concrete is strong in compression, as the aggregate efficiently carries the compression load. However, it is weak in tension as the cement holding the aggregate in place can crack, allowing the structure to fail. Reinforced concrete adds either steel reinforcing bars, steel fibers, glass fibers, or plastic fibers to carry tensile loads.
Chemical admixtures are materials in the form of powder or fluids that are added to the concrete to give it certain characteristics not obtainable with plain concrete mixes. In normal use, admixture dosages are less than 5% by mass of cement and are added to the concrete at the time of batching/mixing. (See § Production below.) The common types of admixtures are as follows:
- Accelerators speed up the hydration (hardening) of the concrete. Typical materials used are CaCl
2, Ca(NO3)2 and NaNO3. However, use of chlorides may cause corrosion in steel reinforcing and is prohibited in some countries, so that nitrates may be favored. Accelerating admixtures are especially useful for modifying the properties of concrete in cold weather.
- Retarders slow the hydration of concrete and are used in large or difficult pours where partial setting before the pour is complete is undesirable. Typical polyol retarders are sugar, sucrose, sodium gluconate, glucose, citric acid, and tartaric acid.
- Air entraining agents add and entrain tiny air bubbles in the concrete, which reduces damage during freeze-thaw cycles, increasing durability. However, entrained air entails a trade off with strength, as each 1% of air may decrease compressive strength by 5%. If too much air becomes trapped in the concrete as a result of the mixing process, Defoamers can be used to encourage the air bubble to agglomerate, rise to the surface of the wet concrete and then disperse.
- Plasticizers increase the workability of plastic, or "fresh", concrete, allowing it to be placed more easily, with less consolidating effort. A typical plasticizer is lignosulfonate. Plasticizers can be used to reduce the water content of a concrete while maintaining workability and are sometimes called water-reducers due to this use. Such treatment improves its strength and durability characteristics. Superplasticizers (also called high-range water-reducers) are a class of plasticizers that have fewer deleterious effects and can be used to increase workability more than is practical with traditional plasticizers. Compounds used as superplasticizers include sulfonated naphthalene formaldehyde condensate, sulfonated melamine formaldehyde condensate, acetone formaldehyde condensate and polycarboxylate ethers.
- Pigments can be used to change the color of concrete, for aesthetics.
- Corrosion inhibitors are used to minimize the corrosion of steel and steel bars in concrete.
- Bonding agents are used to create a bond between old and new concrete (typically a type of polymer) with wide temperature tolerance and corrosion resistance.
- Pumping aids improve pumpability, thicken the paste and reduce separation and bleeding.
Mineral admixtures and blended cementsEdit
|Property||Portland cement||Siliceous[b] fly ash||Calcareous[c] fly ash||Slag cement||Silica fume|
|General use in concrete||Primary binder||Cement replacement||Cement replacement||Cement replacement||Property enhancer|
Inorganic materials that have pozzolanic or latent hydraulic properties, these very fine-grained materials are added to the concrete mix to improve the properties of concrete (mineral admixtures), or as a replacement for Portland cement (blended cements). Products which incorporate limestone, fly ash, blast furnace slag, and other useful materials with pozzolanic properties into the mix, are being tested and used. This development is due to cement production being one of the largest producers (at about 5 to 10%) of global greenhouse gas emissions, as well as lowering costs, improving concrete properties, and recycling wastes.
- Fly ash: A by-product of coal-fired electric generating plants, it is used to partially replace Portland cement (by up to 60% by mass). The properties of fly ash depend on the type of coal burnt. In general, siliceous fly ash is pozzolanic, while calcareous fly ash has latent hydraulic properties.
- Ground granulated blast furnace slag (GGBFS or GGBS): A by-product of steel production is used to partially replace Portland cement (by up to 80% by mass). It has latent hydraulic properties.
- Silica fume: A byproduct of the production of silicon and ferrosilicon alloys. Silica fume is similar to fly ash, but has a particle size 100 times smaller. This results in a higher surface-to-volume ratio and a much faster pozzolanic reaction. Silica fume is used to increase strength and durability of concrete, but generally requires the use of superplasticizers for workability.
- High reactivity Metakaolin (HRM): Metakaolin produces concrete with strength and durability similar to concrete made with silica fume. While silica fume is usually dark gray or black in color, high-reactivity metakaolin is usually bright white in color, making it the preferred choice for architectural concrete where appearance is important.
- Carbon nanofibers can be added to concrete to enhance compressive strength and gain a higher Young’s modulus, and also to improve the electrical properties required for strain monitoring, damage evaluation and self-health monitoring of concrete. Carbon fiber has many advantages in terms of mechanical and electrical properties (e.g., higher strength) and self-monitoring behavior due to the high tensile strength and high conductivity.
- Carbon products have been added to make concrete electrically conductive, for deicing purposes.
Concrete production is the process of mixing together the various ingredients—water, aggregate, cement, and any additives—to produce concrete. Concrete production is time-sensitive. Once the ingredients are mixed, workers must put the concrete in place before it hardens. In modern usage, most concrete production takes place in a large type of industrial facility called a concrete plant, or often a batch plant.
In general usage, concrete plants come in two main types, ready mix plants and central mix plants. A ready-mix plant mixes all the ingredients except water, while a central mix plant mixes all the ingredients including water. A central-mix plant offers more accurate control of the concrete quality through better measurements of the amount of water added, but must be placed closer to the work site where the concrete will be used, since hydration begins at the plant.
A concrete plant consists of large storage hoppers for various reactive ingredients like cement, storage for bulk ingredients like aggregate and water, mechanisms for the addition of various additives and amendments, machinery to accurately weigh, move, and mix some or all of those ingredients, and facilities to dispense the mixed concrete, often to a concrete mixer truck.
Modern concrete is usually prepared as a viscous fluid, so that it may be poured into forms, which are containers erected in the field to give the concrete its desired shape. Concrete formwork can be prepared in several ways, such as Slip forming and Steel plate construction. Alternatively, concrete can be mixed into dryer, non-fluid forms and used in factory settings to manufacture Precast concrete products.
A wide variety of equipment is used for processing concrete, from hand tools to heavy industrial machinery. Whichever equipment builders use, however, the objective is to produce the desired building material; ingredients must be properly mixed, placed, shaped, and retained within time constraints. Any interruption in pouring the concrete can cause the initially placed material to begin to set before the next batch is added on top. This creates a horizontal plane of weakness called a cold joint between the two batches. Once the mix is where it should be, the curing process must be controlled to ensure that the concrete attains the desired attributes. During concrete preparation, various technical details may affect the quality and nature of the product.
When initially mixed, Portland cement and water rapidly form a gel of tangled chains of interlocking crystals, and components of the gel continue to react over time. Initially the gel is fluid, which improves workability and aids in placement of the material, but as the concrete sets, the chains of crystals join into a rigid structure, counteracting the fluidity of the gel and fixing the particles of aggregate in place. During curing, the cement continues to react with the residual water in a process of hydration. In properly formulated concrete, once this curing process has terminated the product has the desired physical and chemical properties. Among the qualities typically desired are mechanical strength, low moisture permeability, and chemical and volumetric stability.
Thorough mixing is essential to produce uniform, high-quality concrete. Therefore, equipment and methods should be capable of effectively mixing concrete materials containing the largest specified aggregate to produce uniform mixtures of the lowest slump practical for the work.
Separate paste mixing has shown that the mixing of cement and water into a paste before combining these materials with aggregates can increase the compressive strength of the resulting concrete. The paste is generally mixed in a high-speed, shear-type mixer at a w/cm (water to cement ratio) of 0.30 to 0.45 by mass. The cement paste premix may include admixtures such as accelerators or retarders, superplasticizers, pigments, or silica fume. The premixed paste is then blended with aggregates and any remaining batch water and final mixing is completed in conventional concrete mixing equipment.
Workability is the ability of a fresh (plastic) concrete mix to fill the form/mold properly with the desired work (vibration) and without reducing the concrete's quality. Workability depends on water content, aggregate (shape and size distribution), cementitious content and age (level of hydration) and can be modified by adding chemical admixtures, like superplasticizer. Raising the water content or adding chemical admixtures increases concrete workability. Excessive water leads to increased bleeding or segregation of aggregates (when the cement and aggregates start to separate), with the resulting concrete having reduced quality. The use of an aggregate blend with an undesirable gradation can result in a very harsh mix design with a very low slump, which cannot readily be made more workable by addition of reasonable amounts of water. An undesirable gradation can mean using a large aggregate that is too large for the size of the formwork, or which has too few smaller aggregate grades to serve to fill the gaps between the larger grades, or using too little or too much sand for the same reason, or using too little water, or too much cement, or even using jagged crushed stone instead of smoother round aggregate such as pebbles. Any combination of these factors and others may result in a mix which is too harsh, i.e., which does not flow or spread out smoothly, is difficult to get into the formwork, and which is difficult to surface finish.
Workability can be measured by the concrete slump test, a simple measure of the plasticity of a fresh batch of concrete following the ASTM C 143 or EN 12350-2 test standards. Slump is normally measured by filling an "Abrams cone" with a sample from a fresh batch of concrete. The cone is placed with the wide end down onto a level, non-absorptive surface. It is then filled in three layers of equal volume, with each layer being tamped with a steel rod to consolidate the layer. When the cone is carefully lifted off, the enclosed material slumps a certain amount, owing to gravity. A relatively dry sample slumps very little, having a slump value of one or two inches (25 or 50 mm) out of one foot (305 mm). A relatively wet concrete sample may slump as much as eight inches. Workability can also be measured by the flow table test.
Slump can be increased by addition of chemical admixtures such as plasticizer or superplasticizer without changing the water-cement ratio. Some other admixtures, especially air-entraining admixture, can increase the slump of a mix.
High-flow concrete, like self-consolidating concrete, is tested by other flow-measuring methods. One of these methods includes placing the cone on the narrow end and observing how the mix flows through the cone while it is gradually lifted.
After mixing, concrete is a fluid and can be pumped to the location where needed.
Concrete must be kept moist during curing in order to achieve optimal strength and durability. During curing hydration occurs, allowing calcium-silicate hydrate (C-S-H) to form. Over 90% of a mix's final strength is typically reached within four weeks, with the remaining 10% achieved over years or even decades. The conversion of calcium hydroxide in the concrete into calcium carbonate from absorption of CO2 over several decades further strengthens the concrete and makes it more resistant to damage. This carbonation reaction, however, lowers the pH of the cement pore solution and can corrode the reinforcement bars.
Hydration and hardening of concrete during the first three days is critical. Abnormally fast drying and shrinkage due to factors such as evaporation from wind during placement may lead to increased tensile stresses at a time when it has not yet gained sufficient strength, resulting in greater shrinkage cracking. The early strength of the concrete can be increased if it is kept damp during the curing process. Minimizing stress prior to curing minimizes cracking. High-early-strength concrete is designed to hydrate faster, often by increased use of cement that increases shrinkage and cracking. The strength of concrete changes (increases) for up to three years. It depends on cross-section dimension of elements and conditions of structure exploitation. Addition of short-cut polymer fibers can improve (reduce) shrinkage-induced stresses during curing and increase early and ultimate compression strength.
Properly curing concrete leads to increased strength and lower permeability and avoids cracking where the surface dries out prematurely. Care must also be taken to avoid freezing or overheating due to the exothermic setting of cement. Improper curing can cause scaling, reduced strength, poor abrasion resistance and cracking.
During the curing period, concrete is ideally maintained at controlled temperature and humidity. To ensure full hydration during curing, concrete slabs are often sprayed with "curing compounds" that create a water-retaining film over the concrete. Typical films are made of wax or related hydrophobic compounds. After the concrete is sufficiently cured, the film is allowed to abrade from the concrete through normal use.
Traditional conditions for curing involve by spraying or ponding the concrete surface with water. The adjacent picture shows one of many ways to achieve this, ponding—submerging setting concrete in water and wrapping in plastic to prevent dehydration. Additional common curing methods include wet burlap and plastic sheeting covering the fresh concrete.
For higher-strength applications, accelerated curing techniques may be applied to the concrete. A common technique involves heating the poured concrete with steam, which serves to both keep it damp and raise the temperature, so that the hydration process proceeds more quickly and more thoroughly.
Pervious concrete is a mix of specially graded coarse aggregate, cement, water and little-to-no fine aggregates. This concrete is also known as "no-fines" or porous concrete. Mixing the ingredients in a carefully controlled process creates a paste that coats and bonds the aggregate particles. The hardened concrete contains interconnected air voids totaling approximately 15 to 25 percent. Water runs through the voids in the pavement to the soil underneath. Air entrainment admixtures are often used in freeze–thaw climates to minimize the possibility of frost damage.
Nanoconcrete contains Portland cement particles that are no greater than 100 μm. It is a product of high-energy mixing (HEM) of cement, sand and water. To ensure the mixing is thorough enough to create nanoconcrete, the mixer must apply a total mixing power to the mixture of 30–600 watts per kilogram of the mix. This mixing must continue long enough to yield a net specific energy expended upon the mix of at least 5000 joules per kilogram of the mix.[irrelevant citation] and may be increased to 30–80 kJ per kilogram. A superplasticizer is then added to the activated mixture which can later be mixed with aggregates in a conventional concrete mixer. In the HEM process, the intense mixing of cement and water with sand provides dissipation and absorption of energy by the mixture and increases shear stresses on the surface of cement particles. As a result, the temperature of the mixture increases by 20–25 degrees Celsius. This intense mixing serves to deepen hydration process inside the cement particles. The nano-sized colloid Calcium Silicate Hydrate (C-S-H) formation increased several times compared with conventional mixing. Thus, the ordinary concrete transforms to nanoconcrete. The initial natural process of cement hydration with formation of colloidal globules about 5 nm in diameter spreads into the entire volume of cement–water matrix as the energy expended upon the mix. The liquid activated high-energy mixture can be used by itself for casting small architectural details and decorative items, or foamed (expanded) for lightweight concrete. HEM Nanoconcrete hardens in low and subzero temperature conditions because the liquid phase inside the nano-pores of C-S-H gel doesn't freeze at temperatures from −8 to −42 degrees Celsius. The increased volume of gel reduces capillarity in solid and porous materials.
Bacteria such as Bacillus pasteurii, Bacillus pseudofirmus, Bacillus cohnii, Sporosarcina pasteuri, and Arthrobacter crystallopoietes increase the compression strength of concrete through their biomass. Not all bacteria increase the strength of concrete significantly with their biomass.:143 Bacillus sp. CT-5. can reduce corrosion of reinforcement in reinforced concrete by up to four times. Sporosarcina pasteurii reduces water and chloride permeability. B. pasteurii increases resistance to acid.:146 Bacillus pasteurii and B. sphaericuscan induce calcium carbonate precipitation in the surface of cracks, adding compression strength.:147
Polymer concretes are mixtures of aggregate and any of various polymers and may be reinforced. The cement is costlier than lime-based cements, but polymer concretes nevertheless have advantages; they have significant tensile strength even without reinforcement, and they are largely impervious to water. Polymer concretes are frequently used for repair and construction of other applications, such as drains.
Grinding of concrete can produce hazardous dust. Exposure to cement dust can lead to issues such as silicosis, kidney disease, skin irritation and similar effects. The National Institute for Occupational Safety and Health in the United States recommends attaching local exhaust ventilation shrouds to electric concrete grinders to control the spread of this dust. In addition, the Occupational Safety and Health Administration (OSHA) has placed more stringent regulations on companies whose workers regularly come into contact with silica dust. An updated silica rule, which OSHA put into effect 23 Sept. 2017 for construction companies, restricted the amount of respirable crystalline silica workers could legally come into contact with to 50 micrograms per cubic meter of air per 8-hour workday. That same rule went into effect 23 June 2018 for general industry, hydraulic fracturing and maritime. It should be noted, however, that the deadline was extended to 23 June 2021 for engineering controls in the hydraulic fracturing industry. Companies which fail to meet the tightened safety regulations can face financial charges and extensive penalties.
Cement dust is not the only concern crews face when working with concrete. Improper ergonomics can lead to muscle pains and strains. As such, it is important for crews to practice proper stretching before embarking on a busy workday. Working in close quarters can also place team members in danger. Not only can crowded workspaces make it difficult for crews to safely exit, but certain work environments—such as jobs carried out inside cement mixing drums—make ventilation an obstacle. Furthermore, crews who carry out much of their work outdoors face weather-related concerns. It is important for crews to take special precautions when faced with extremely hot conditions and cold conditions. Such is the case for all outdoor crews, whether they work with concrete or not.
Concrete has relatively high compressive strength, but much lower tensile strength. Therefore, it is usually reinforced with materials that are strong in tension (often steel). The elasticity of concrete is relatively constant at low stress levels but starts decreasing at higher stress levels as matrix cracking develops. Concrete has a very low coefficient of thermal expansion and shrinks as it matures. All concrete structures crack to some extent, due to shrinkage and tension. Concrete that is subjected to long-duration forces is prone to creep.
Tests can be performed to ensure that the properties of concrete correspond to specifications for the application.
Different mixes of concrete ingredients produce different strengths. Concrete strength values are usually specified as the lower-bound compressive strength of either a cylindrical or cubic specimen as determined by standard test procedures.
Different strengths of concrete are used for different purposes. Very low-strength—14 MPa (2,000 psi) or less—concrete may be used when the concrete must be lightweight. Lightweight concrete is often achieved by adding air, foams, or lightweight aggregates, with the side effect that the strength is reduced. For most routine uses, 20 MPa (2,900 psi) to 32 MPa (4,600 psi) concrete is often used. 40 MPa (5,800 psi) concrete is readily commercially available as a more durable, although more expensive, option. Higher-strength concrete is often used for larger civil projects. Strengths above 40 MPa (5,800 psi) are often used for specific building elements. For example, the lower floor columns of high-rise concrete buildings may use concrete of 80 MPa (11,600 psi) or more, to keep the size of the columns small. Bridges may use long beams of high-strength concrete to lower the number of spans required. Occasionally, other structural needs may require high-strength concrete. If a structure must be very rigid, concrete of very high strength may be specified, even much stronger than is required to bear the service loads. Strengths as high as 130 MPa (18,900 psi) have been used commercially for these reasons.
Concrete is one of the most durable building materials. It provides superior fire resistance compared with wooden construction and gains strength over time. Structures made of concrete can have a long service life. Concrete is used more than any other artificial material in the world. As of 2006, about 7.5 billion cubic meters of concrete are made each year, more than one cubic meter for every person on Earth.
Due to cement's exothermic chemical reaction while setting up, large concrete structures such as dams, navigation locks, large mat foundations, and large breakwaters generate excessive heat during hydration and associated expansion. To mitigate these effects post-cooling is commonly applied during construction. An early example at Hoover Dam used a network of pipes between vertical concrete placements to circulate cooling water during the curing process to avoid damaging overheating. Similar systems are still used; depending on volume of the pour, the concrete mix used, and ambient air temperature, the cooling process may last for many months after the concrete is placed. Various methods also are used to pre-cool the concrete mix in mass concrete structures.
Another approach to mass concrete structures that minimizes cement's thermal byproduct is the use of roller-compacted concrete, which uses a dry mix which has a much lower cooling requirement than conventional wet placement. It is deposited in thick layers as a semi-dry material then roller compacted into a dense, strong mass.
Raw concrete surfaces tend to be porous and have a relatively uninteresting appearance. Many different finishes can be applied to improve the appearance and preserve the surface against staining, water penetration, and freezing.
Examples of improved appearance include stamped concrete where the wet concrete has a pattern impressed on the surface, to give a paved, cobbled or brick-like effect, and may be accompanied with coloration. Another popular effect for flooring and table tops is polished concrete where the concrete is polished optically flat with diamond abrasives and sealed with polymers or other sealants.
Other finishes can be achieved with chiseling, or more conventional techniques such as painting or covering it with other materials.
The proper treatment of the surface of concrete, and therefore its characteristics, is an important stage in the construction and renovation of architectural structures.
Prestressed concrete is a form of reinforced concrete that builds in compressive stresses during construction to oppose tensile stresses experienced in use. This can greatly reduce the weight of beams or slabs, by better distributing the stresses in the structure to make optimal use of the reinforcement. For example, a horizontal beam tends to sag. Prestressed reinforcement along the bottom of the beam counteracts this. In pre-tensioned concrete, the prestressing is achieved by using steel or polymer tendons or bars that are subjected to a tensile force prior to casting, or for post-tensioned concrete, after casting.
More than 55,000 miles (89,000 km) of highways in the United States are paved with this material. Reinforced concrete, prestressed concrete and precast concrete are the most widely used types of concrete functional extensions in modern days. See Brutalism.
Cold weather placementEdit
Extreme weather conditions (extreme heat or cold; windy condition, and humidity variations) can significantly alter the quality of concrete. Many precautions are observed in cold weather placement. Low temperatures significantly slow the chemical reactions involved in hydration of cement, thus affecting the strength development. Preventing freezing is the most important precaution, as formation of ice crystals can cause damage to the crystalline structure of the hydrated cement paste. If the surface of the concrete pour is insulated from the outside temperatures, the heat of hydration will prevent freezing.
- A period when for more than three successive days the average daily air temperature drops below 40 ˚F (~ 4.5 °C), and
- Temperature stays below 50 ˚F (10 °C) for more than one-half of any 24-hour period.
In Canada, where temperatures tend to be much lower during the cold season, the following criteria are used by CSA A23.1:
- When the air temperature is ≤ 5 °C, and
- When there is a probability that the temperature may fall below 5 °C within 24 hours of placing the concrete.
The minimum strength before exposing concrete to extreme cold is 500 psi (3.5 MPa). CSA A 23.1 specified a compressive strength of 7.0 MPa to be considered safe for exposure to freezing.
Concrete roads are more fuel efficient to drive on, more reflective and last significantly longer than other paving surfaces, yet have a much smaller market share than other paving solutions. Modern-paving methods and design practices have changed the economics of concrete paving, so that a well-designed and placed concrete pavement will be less expensive on initial costs and significantly less expensive over the life cycle. Another major benefit is that pervious concrete can be used, which eliminates the need to place storm drains near the road, and reducing the need for slightly sloped roadway to help rainwater to run off. No longer requiring discarding rainwater through use of drains also means that less electricity is needed (more pumping is otherwise needed in the water-distribution system), and no rainwater gets polluted as it no longer mixes with polluted water. Rather, it is immediately absorbed by the ground.
Energy requirements for transportation of concrete are low because it is produced locally from local resources, typically manufactured within 100 kilometers of the job site. Similarly, relatively little energy is used in producing and combining the raw materials (although large amounts of CO2 are produced by the chemical reactions in cement manufacture). The overall embodied energy of concrete at roughly 1 to 1.5 megajoules per kilogram is therefore lower than for most structural and construction materials.
Once in place, concrete offers great energy efficiency over the lifetime of a building. Concrete walls leak air far less than those made of wood frames. Air leakage accounts for a large percentage of energy loss from a home. The thermal mass properties of concrete increase the efficiency of both residential and commercial buildings. By storing and releasing the energy needed for heating or cooling, concrete's thermal mass delivers year-round benefits by reducing temperature swings inside and minimizing heating and cooling costs. While insulation reduces energy loss through the building envelope, thermal mass uses walls to store and release energy. Modern concrete wall systems use both external insulation and thermal mass to create an energy-efficient building. Insulating concrete forms (ICFs) are hollow blocks or panels made of either insulating foam or rastra that are stacked to form the shape of the walls of a building and then filled with reinforced concrete to create the structure.
Concrete buildings are more resistant to fire than those constructed using steel frames, since concrete has lower heat conductivity than steel and can thus last longer under the same fire conditions. Concrete is sometimes used as a fire protection for steel frames, for the same effect as above. Concrete as a fire shield, for example Fondu fyre, can also be used in extreme environments like a missile launch pad.
Options for non-combustible construction include floors, ceilings and roofs made of cast-in-place and hollow-core precast concrete. For walls, concrete masonry technology and Insulating Concrete Forms (ICFs) are additional options. ICFs are hollow blocks or panels made of fireproof insulating foam that are stacked to form the shape of the walls of a building and then filled with reinforced concrete to create the structure.
Concrete also provides good resistance against externally applied forces such as high winds, hurricanes, and tornadoes owing to its lateral stiffness, which results in minimal horizontal movement. However, this stiffness can work against certain types of concrete structures, particularly where a relatively higher flexing structure is required to resist more extreme forces.
As discussed above, concrete is very strong in compression, but weak in tension. Larger earthquakes can generate very large shear loads on structures. These shear loads subject the structure to both tensile and compressional loads. Concrete structures without reinforcement, like other unreinforced masonry structures, can fail during severe earthquake shaking. Unreinforced masonry structures constitute one of the largest earthquake risks globally. These risks can be reduced through seismic retrofitting of at-risk buildings, (e.g. school buildings in Istanbul, Turkey).
Concrete can be damaged by many processes, such as the expansion of corrosion products of the steel reinforcement bars, freezing of trapped water, fire or radiant heat, aggregate expansion, sea water effects, bacterial corrosion, leaching, erosion by fast-flowing water, physical damage and chemical damage (from carbonatation, chlorides, sulfates and distillate water). The micro fungi Aspergillus Alternaria and Cladosporium were able to grow on samples of concrete used as a radioactive waste barrier in the Chernobyl reactor; leaching aluminum, iron, calcium, and silicon.
Effect of modern useEdit
Concrete is widely used for making architectural structures, foundations, brick/block walls, pavements, bridges/overpasses, highways, runways, parking structures, dams, pools/reservoirs, pipes, footings for gates, fences and poles and even boats. Concrete is used in large quantities almost everywhere there is a need for infrastructure. Concrete is one of the most frequently used building materials in animal houses and for manure and silage storage structures in agriculture.
The amount of concrete used worldwide, ton for ton, is twice that of steel, wood, plastics, and aluminum combined. Concrete's use in the modern world is exceeded only by that of naturally occurring water.
Concrete is also the basis of a large commercial industry. Globally, the ready-mix concrete industry, the largest segment of the concrete market, is projected to exceed $600 billion in revenue by 2025. In the United States alone, concrete production is a $30-billion-per-year industry, considering only the value of the ready-mixed concrete sold each year. Given the size of the concrete industry, and the fundamental way concrete is used to shape the infrastructure of the modern world, it is difficult to overstate the role this material plays today.
Environmental and healthEdit
The manufacture and use of concrete produce a wide range of environmental and social consequences. Some are harmful, some welcome, and some both, depending on circumstances.
A major component of concrete is cement, which similarly exerts environmental and social effects.:142 The cement industry is one of the three primary producers of carbon dioxide, a major greenhouse gas (the other two being the energy production and transportation industries). Every tonne of cement produced releases one tonne of CO2 into the atmosphere. As of 2019, the production of Portland cement contributed eight percent to global anthropogenic CO2 emissions, largely due to the sintering of limestone and clay at 1,500 °C (2,730 °F). Researchers have suggested a number of approaches to improving carbon sequestration relevant to concrete production.
Concrete is used to create hard surfaces that contribute to surface runoff, which can cause heavy soil erosion, water pollution, and flooding, but conversely can be used to divert, dam, and control flooding. Concrete dust released by building demolition and natural disasters can be a major source of dangerous air pollution.
Workers who cut, grind or polish concrete are at risk of inhaling airborne silica, which can lead to silicosis. This includes crew members who work in concrete chipping. The presence of some substances in concrete, including useful and unwanted additives, can cause health concerns due to toxicity and radioactivity. Fresh concrete (before curing is complete) is highly alkaline and must be handled with proper protective equipment.
Concrete recycling is an increasingly common method for disposing of concrete structures. Concrete debris was once routinely shipped to landfills for disposal, but recycling is increasing due to improved environmental awareness, governmental laws and economic benefits.
Reinforced concrete contains rebar and other metallic reinforcements, which are removed with magnets and recycled elsewhere. The remaining aggregate chunks are sorted by size. Larger chunks may go through the crusher again. Smaller pieces of concrete are used as gravel for new construction projects. Aggregate base gravel is laid down as the lowest layer in a road, with fresh concrete or asphalt placed over it. Crushed recycled concrete can sometimes be used as the dry aggregate for brand new concrete if it is free of contaminants, though the use of recycled concrete limits strength and is not allowed in many jurisdictions. On 3 March 1983, a government-funded research team (the VIRL research.codep) estimated that almost 17% of worldwide landfill was by-products of concrete based waste.
It is important to note that, as with concrete chipping, polishing and similar work, the process of recycling concrete can expose workers to dangerous silica dust. A recent silica rule update  set forth by the Occupational Safety and Health Administration (OSHA) limits the legal amount of respirable crystalline silica workers can come in contact with to 50 micrograms per cubic meter of air per 8-hour workday.
Concrete chipping is the act of breaking away the dried concrete that forms along the walls of central mixers and ready-mix concrete trucks. Whenever possible, teams carry out the work by physically entering the spaces and breaking away the dried material with help from handheld jackhammers and chisels. Once removed, the broken concrete is either hauled away to landfills, recycled or reused in some other way.
While specific concrete chipping needs vary by fleet size, concrete blends at play and the specific drums in use, it is generally accepted that a company should have its drums chipped every three months. Such maintenance helps companies avoid slowdowns in production, lowered drum capacity and breakdowns which can affect their bottom line.
As with all concrete work, concrete chipping carries its share of on-the-job dangers. Silica dust exposure, cramped quarters, flying debris and other hazards are all concerns team members can face at work. Regular training, as well as adherence to regulations set forth by the Occupational Safety and Health Administration (OSHA) help keep team members safe.
The world record for the largest concrete pour in a single project is the Three Gorges Dam in Hubei Province, China by the Three Gorges Corporation. The amount of concrete used in the construction of the dam is estimated at 16 million cubic meters over 17 years. The previous record was 12.3 million cubic meters held by Itaipu hydropower station in Brazil.
The world record for concrete pumping was set on 7 August 2009 during the construction of the Parbati Hydroelectric Project, near the village of Suind, Himachal Pradesh, India, when the concrete mix was pumped through a vertical height of 715 m (2,346 ft).
The world record for the largest continuously poured concrete raft was achieved in August 2007 in Abu Dhabi by contracting firm Al Habtoor-CCC Joint Venture and the concrete supplier is Unibeton Ready Mix. The pour (a part of the foundation for the Abu Dhabi's Landmark Tower) was 16,000 cubic meters of concrete poured within a two-day period. The previous record, 13,200 cubic meters poured in 54 hours despite a severe tropical storm requiring the site to be covered with tarpaulins to allow work to continue, was achieved in 1992 by joint Japanese and South Korean consortiums Hazama Corporation and the Samsung C&T Corporation for the construction of the Petronas Towers in Kuala Lumpur, Malaysia.
The world record for largest continuously poured concrete floor was completed 8 November 1997, in Louisville, Kentucky by design-build firm EXXCEL Project Management. The monolithic placement consisted of 225,000 square feet (20,900 m2) of concrete placed in 30 hours, finished to a flatness tolerance of FF 54.60 and a levelness tolerance of FL 43.83. This surpassed the previous record by 50% in total volume and 7.5% in total area.
The record for the largest continuously placed underwater concrete pour was completed 18 October 2010, in New Orleans, Louisiana by contractor C. J. Mahan Construction Company, LLC of Grove City, Ohio. The placement consisted of 10,251 cubic yards of concrete placed in 58.5 hours using two concrete pumps and two dedicated concrete batch plants. Upon curing, this placement allows the 50,180-square-foot (4,662 m2) cofferdam to be dewatered approximately 26 feet (7.9 m) below sea level to allow the construction of the Inner Harbor Navigation Canal Sill & Monolith Project to be completed in the dry.
- Concrete portal
- Anthropic rock
- Brutalist architecture
- Cement accelerator
- Concrete canoe
- Concrete chipping
- Concrete leveling
- Concrete mixer
- Concrete masonry unit
- Concrete moisture meter
- Concrete plant
- Concrete recycling
- Concrete step barrier
- Concrete sealers
- Diamond grinding of pavement
- Foam Index
- Form liner
- High performance fiber reinforced cementitious composites
- International Grooving & Grinding Association
- Lift Slab Construction
- Rammed earth
- Rusticated concrete block
- Shallow foundation
- Silica fume
- Translucent concrete
- World of Concrete
- The Roman Pantheon: The Triumph of Concrete Archived 6 October 2014 at the Wayback Machine. Romanconcrete.com. Retrieved on 2013-02-19.
- Industrial Resources Council (2008). "Portland Cement Concrete". www.industrialresourcescouncil.org. Retrieved 2018-06-15.
- National Highway Institute. "Portland Cement Concrete Materials" (PDF). Federal Highway Administration.
- Zongjin Li; Advanced concrete technology; 2011
- Moore, David (1999). "The Pantheon". romanconcrete.com. Archived from the original on 1 October 2011. Retrieved 26 September 2011.
- Smil, Vaclav (2016-12-04). Making the Modern World: Materials and Dematerialization. Lulu Press, Inc. ISBN 9781365581908.
- "concretus". Latin Lookup. Archived from the original on 12 May 2013. Retrieved 1 October 2012.
- Gromicko, Nick; Shepard, Kenton (2016). "The History of Concrete". International Association of Certified Home Inspectors, Inc. Retrieved 2018-12-27.
- Heinrich Schliemann; Wilhelm Dörpfeld; Felix Adler (1885). Tiryns: The Prehistoric Palace of the Kings of Tiryns, the Results of the Latest Excavations. New York, New York: Charles Scribner's Sons. pp. 190, 203, 204, 215.
- Amelia Carolina Sparavigna, "Ancient concrete works"
- Jacobsen T and Lloyd S, (1935) "Sennacherib's Aqueduct at Jerwan," Oriental Institute Publications 24, Chicago University Press
- Stella L. Marusin (1 January 1996). "Ancient Concrete Structures". Concrete International. 18 (1): 56–58.
- "The History of Concrete". Dept. of Materials Science and Engineering, University of Illinois, Urbana-Champaign. Archived from the original on 27 November 2012. Retrieved 8 January 2013.
- Lancaster, Lynne (2005). Concrete Vaulted Construction in Imperial Rome. Innovations in Context. Cambridge University Press. ISBN 978-0-511-16068-4.
- D.S. Robertson: Greek and Roman Architecture, Cambridge, 1969, p. 233
- Henry Cowan: The Masterbuilders, New York 1977, p. 56, ISBN 978-0-471-02740-9
- History of Concrete Archived 27 February 2017 at the Wayback Machine
- Robert Mark, Paul Hutchinson: "On the Structure of the Roman Pantheon", Art Bulletin, Vol. 68, No. 1 (1986), p. 26, fn. 5
- Jackson, Marie D.; Landis, Eric N.; Brune, Philip F.; Vitti, Massimo; Chen, Heng; Li, Qinfei; Kunz, Martin; Wenk, Hans-Rudolf; Monteiro, Paulo J. M.; Ingraffea, Anthony R. (30 December 2014). "Mechanical resilience and cementitious processes in Imperial Roman architectural mortar". PNAS. 111 (52): 18484–18489. Bibcode:2014PNAS..11118484J. doi:10.1073/pnas.1417456111. PMC 4284584. PMID 25512521.
- Marie D. Jackson, Sean R. Mulcahy, Heng Chen, Yao Li, Qinfei Li, Piergiulio Cappelletti, Hans-Rudolf Wenk (3 July 2017). "Phillipsite and Al-tobermorite mineral cements produced through low-temperature water-rock reactions in Roman marine concrete". American Mineralogist. 102 (7): 1435–1450. Bibcode:2017AmMin.102.1435J. doi:10.2138/am-2017-5993CCBY. Archived from the original on 5 July 2017.CS1 maint: Uses authors parameter (link)
- "Secret of how Roman concrete survived tidal battering for 2,000 years revealed". The Telegraph. Archived from the original on 4 July 2017.
- "The Politics of Rediscovery in the History of Science: Tacit Knowledge of Concrete before its Discovery". Archived from the original on 5 May 2010. Retrieved 14 January 2010.CS1 maint: BOT: original-url status unknown (link). allacademic.com
- Nick Gromicko & Kenton Shepard. "the History of Concrete". The International Association of Certified Home Inspectors (InterNACHI). Archived from the original on 15 January 2013. Retrieved 8 January 2013.
- Herring, Benjamin. "The Secrets of Roman Concrete" (PDF). Romanconcrete.com. Archived (PDF) from the original on 15 September 2012. Retrieved 1 October 2012.
- Courland, Robert (2011). Concrete planet : the strange and fascinating story of the world's most common man-made material. Amherst, N.Y.: Prometheus Books. ISBN 978-1616144814. Archived from the original on 4 November 2015. Retrieved 28 August 2015.
- The History of Concrete and Cement. Inventors.about.com (2012-04-09). Retrieved on 2013-02-19.
- "Francois Coignet - French house builder". Retrieved 23 December 2016.
- « Château de Chazelet » [archive], notice no PA00097319, base Mérimée, ministère français de la Culture.
- Evelien Cochez; Wouter Nijs; Giorgio Simbolotti & Giancarlo Tosato. "Cement Production" (PDF). IEA ETSAP, Technology Brief I03, June 2010: IEA ETSAP- Energy Technology Systems Analysis Programme. Archived from the original (PDF) on 24 January 2013. Retrieved 9 January 2013.
- Gibbons, Jack. "Measuring Water in Concrete". Concrete Construction. Archived from the original on 11 May 2013. Retrieved 1 October 2012.
- "CHAPTER 9 Designing and Proportioning Normal Concrete Mixtures" (PDF). PCA manual. Portland Concrete Association. Archived (PDF) from the original on 26 May 2012. Retrieved 1 October 2012.
- Taha, Ramzi A. "Use of Production and Brackish Water in Concrete Mixtures" (PDF). International Journal of Sustainable Water and Environmental System. Retrieved 1 October 2012.[permanent dead link]
- "Cement hydration". Understanding Cement. Archived from the original on 17 October 2012. Retrieved 1 October 2012.
- The Effect of Aggregate Properties on Concrete Archived 25 December 2012 at the Wayback Machine. Engr.psu.edu. Retrieved on 2013-02-19.
- Veretennykov, Vitaliy I.; Yugov, Anatoliy M.; Dolmatov, Andriy O.; Bulavytskyi, Maksym S.; Kukharev, Dmytro I.; Bulavytskyi, Artem S. (2008). "Concrete Inhomogeneity of Vertical Cast-in-Place Elements in Skeleton-Type Buildings" (PDF). In Mohammed Ettouney. AEI 2008: Building Integration Solutions. Reston, Virginia: American Society of Civil Engineers. doi:10.1061/41002(328)17. ISBN 978-0-7844-1002-8. Archived (PDF) from the original on 3 April 2015. Retrieved 25 December 2010.
- Exposed Aggregate Archived 12 January 2013 at the Wayback Machine. Uniquepaving.com.au. Retrieved on 2013-02-19.
- U.S. Federal Highway Administration (14 June 1999). "Admixtures". Archived from the original on 27 January 2007. Retrieved 25 January 2007.
- Cement Admixture Association. "Admixture Types". Archived from the original on 3 September 2011. Retrieved 25 December 2010.
- "Archived copy". Archived from the original on 1 December 2016. Retrieved 15 January 2017.CS1 maint: Archived copy as title (link)
- Holland, Terence C. (2005). "Silica Fume User's Manual" (PDF). Silica Fume Association and United States Department of Transportation Federal Highway Administration Technical Report FHWA-IF-05-016. Retrieved October 31, 2014.
- Kosmatka, S.; Kerkhoff, B.; Panerese, W. (2002). Design and Control of Concrete Mixtures (14 ed.). Portland Cement Association, Skokie, Illinois.
- Gamble, William. "Cement, Mortar, and Concrete". In Baumeister; Avallone; Baumeister. Mark's Handbook for Mechanical Engineers (Eighth ed.). McGraw Hill. Section 6, page 177.
- Kosmatka, S.H.; Panarese, W.C. (1988). Design and Control of Concrete Mixtures. Skokie, IL, USA: Portland Cement Association. pp. 17, 42, 70, 184. ISBN 978-0-89312-087-0.
- Paving the way to greenhouse gas reductions Archived 31 October 2012 at the Wayback Machine. Web.mit.edu (2011-08-28). Retrieved on 2013-02-19.
- U.S. Federal Highway Administration (14 June 1999). "Fly Ash". Archived from the original on 10 July 2007. Retrieved 24 January 2007.
- U.S. Federal Highway Administration. "Ground Granulated Blast-Furnace Slag". Archived from the original on 22 January 2007. Retrieved 24 January 2007.
- U.S. Federal Highway Administration. "Silica Fume". Archived from the original on 22 January 2007. Retrieved 24 January 2007.
- Mullapudi, Taraka Ravi Shankar; Gao, Di; Ayoub, Ashraf (1 September 2013). "Non-destructive evaluation of carbon nanofibre concrete". Magazine of Concrete Research. 65 (18): 1081–1091. doi:10.1680/macr.12.00187.
- "Evaluation of Electrically Conductive Concrete Containing Carbon Products for Deicing" (PDF). ACI Materials Journal. Archived from the original (PDF) on 10 May 2013. Retrieved 1 October 2012.
- Cold Joints Archived 4 March 2016 at the Wayback Machine, The Concrete Society, accessed 2015-12-30
- Premixed cement paste Archived 28 September 2007 at the Wayback Machine. Concreteinternational.com (1989-11-01). Retrieved on 2013-02-19.
- "ACI 304R-00: Guide for Measuring, Mixing, Transporting, and Placing Concrete (Reapproved 2009)".
- "Archived copy". Archived from the original on 16 January 2017. Retrieved 15 January 2017.CS1 maint: Archived copy as title (link)
- "Archived copy". Archived from the original on 2 February 2017. Retrieved 15 January 2017.CS1 maint: Archived copy as title (link)
- Ferrari, L; Kaufmann, J; Winnefeld, F; Plank, J (2011). "Multi-method approach to study influence of superplasticizers on cement suspensions". Cement and Concrete Research. 41 (10): 1058. doi:10.1016/j.cemconres.2011.06.010.
- "Curing Concrete" Peter C. Taylor CRC Press 2013. ISBN 978-0-415-77952-4. eBook ISBN 978-0-203-86613-9
- "Concrete Testing". Archived from the original on 24 October 2008. Retrieved 10 November 2008.
- Resulting strength distribution in vertical elements researched and presented at the article "Concrete inhomogeneity of vertical cast-in-place elements in skeleton-type buildings". Archived 3 April 2015 at the Wayback Machine
- "Admixtures for Cementitious Applications." Archived 17 October 2016 at the Wayback Machine
- "Archived copy" (PDF). Archived (PDF) from the original on 8 December 2015. Retrieved 12 November 2015.CS1 maint: Archived copy as title (link)
- Tiwari, AK; Chowdhury, Subrato (2013). "An over view of the application of nanotechnology in construction materials". Proceedings of the International Symposium on Engineering under Uncertainty: Safety Assessment and Management (ISEUSAM-2012). Cakrabartī, Subrata., Bhattacharya, Gautam. New Delhi: Springer India. p. 485. ISBN 9788132207573. OCLC 831413888.
- Fridman, Vladen (22 August 1995). "Method for producing Construction Mixture for concrete patent number: 5,443,313".
- Raki, Laila; Beaudoin, James; Alizadeh, Rouhollah; Makar, Jon; Sato, Taijiro (2010). "Cement and Concrete Nanoscience and Nanotechnology". Materials. 3 (2): 918–942. Bibcode:2010Mate....3..918R. doi:10.3390/ma3020918. ISSN 1996-1944. Archived from the original on 15 March 2015.
- Fridman, Vladen (March 1, 2018). "NANOCONCRETE".
- R.A. Olson; et al. (1995). "Interpretation of the impedance spectroscopy of cement paste via computer modeling. Part III Microstructural analysis of frozen cement paste". Journal of Materials Science. 30: 5081.
- General Chipping. "How Do I Protect My Team and Those Around Them from Cement Dust?", General Chipping. Retrieved on 5 November 2018.
- "CDC - NIOSH Publications and Products - Control of Hazardous Dust When Grinding Concrete (2009-115)". www.cdc.gov. Archived from the original on 20 August 2016. Retrieved 13 July 2016.
- OSHA Fact Sheet. "OSHA’s Respirable Crystalline Silica Standard for General Industry and Maritime", Occupational Safety and Health Administration. Retrieved on 5 November 2018.
- General Chipping. "Safety at the Forefront: Ergonomics in Concrete Work", General Chipping. Retrieved on 5 November 2018.
- General Chipping. "Why (and How) You Should Stretch Before Strenuous Physical Work", General Chipping. Retrieved on 5 November 2018.
- General Chipping. "Confined Spaces: Understanding the Hazards of Concrete Chipping", General Chipping. Retrieved on 5 November 2018.
- General Chipping. "How Can I Protect My Team During Hot Summer Months?", General Chipping. Retrieved on 5 November 2018.
- General Chipping. "How Can I Encourage Cold Weather Safety for My Crew?", General Chipping. Retrieved on 5 November 2018.
- "Structural lightweight concrete" (PDF). Concrete Construction. The Aberdeen Group. March 1981. Archived from the original (PDF) on 11 May 2013.
- "Ordering Concrete by PSI". American Concrete. Archived from the original on 11 May 2013. Retrieved 10 January 2013.
- Henry G. Russel, PE. "Why Use High Performance Concrete?" (PDF). Technical Talk. Archived (PDF) from the original on 15 May 2013. Retrieved 10 January 2013.
- "Concrete in Practice: What, Why, and How?" (PDF). NRMCA-National Ready Mixed Concrete Association. Archived (PDF) from the original on 4 August 2012. Retrieved 10 January 2013.
- Lomborg, Bjørn (2001). The Skeptical Environmentalist: Measuring the Real State of the World. p. 138. ISBN 978-0-521-80447-9.
- "Minerals commodity summary – cement – 2007". US United States Geological Survey. 1 June 2007. Archived from the original on 13 December 2007. Retrieved 16 January 2008.
- Mass Concrete Archived 27 September 2011 at the Wayback Machine. (PDF) . Retrieved on 2013-02-19.
- ^ Sadowski, Łukasz; Mathia, Thomas. "Multi-scale Metrology of Concrete Surface Morphology: Fundamentals and specificity". Construction and Building Materials 113: 613–621. doi:http:// doi:10.1016/j.conbuildmat.2016.03.099
- "Winter is Coming! Precautions for Cold Weather Concreting | FPrimeC Solutions". FPrimeC Solutions. 14 November 2016. Archived from the original on 13 January 2017. Retrieved 11 January 2017.
- "306R-16 Guide to Cold Weather Concreting". Archived from the original on 15 September 2017.
- "Mapping of Excess Fuel Consumption". Archived from the original on 2 January 2015.
- Rubenstein, Madeleine. "Emissions from the Cement Industry". State of the Planet. Earth Institute, Columbia University. Archived from the original on 22 December 2016. Retrieved 13 December 2016.
- "Archived copy". Archived from the original on 16 January 2017. Retrieved 15 January 2017.CS1 maint: Archived copy as title (link)
- John Gajda (2001) Energy Use of Single Family Houses with Various Exterior Walls, Construction Technology Laboratories Inc.
- Green Building with Concrete. Taylor & Francis Group. 2015-06-16. ISBN 978-1-4987-0411-3.
- "Features and Usage of Foam Concrete". Archived from the original on 29 November 2012.
- Unreinforced Masonry Buildings and Earthquakes: Developing Successful Risk Reduction Programs Archived 12 September 2011 at the Wayback Machine, FEMA P-774 / October 2009
- Seismic Retrofit Design Of Historic Century-Old School Buildings In Istanbul, Turkey Archived 11 January 2012 at the Wayback Machine, C.C. Simsir, A. Jain, G.C. Hart, and M.P. Levy, The 14th World Conference on Earthquake Engineering, 12–17 October 2008, Beijing, China
- Luis Emilio Rendon Diaz Miron; Dessi A. Koleva (27 April 2017). Concrete Durability: Cementitious Materials and Reinforced Concrete Properties, Behavior and Corrosion Resistance. Springer. pp. 2–. ISBN 978-3-319-55463-1.
- Geoffrey Michael Gadd (March 2010). "Metals, minerals and microbes: geomicrobiology and bioremediation". Microbiology. 156 (Pt 3): 609–643. doi:10.1099/mic.0.037143-0. PMID 20019082. Archived from the original on 25 October 2014.
- De Belie, Nele (2000). "Durability of Building Materials and Components in the Agricultural Environment, Part III: Concrete Structures". J. Agric. Engng Res.
- "What is the development impact of concrete?". Cement Trust. Archived from the original on 17 September 2012. Retrieved 10 January 2013.
- Vidal, John (2019-02-25). "Concrete is tipping us into climate catastrophe. It's payback time". The Guardian. Retrieved 2019-02-27.
- Worrell, E.; Price, L.; Martin, N.; Hendriks, C.; Ozawa Meida, L. (2001). "Carbon dioxide emissions from the global cement industry". Annu. Rev. Energy Environ. 26: 303–329. doi:10.1146/annurev.energy.26.1.303. Cited in
- Rinde, Meir (2017). "Concrete Solutions". Distillations. 3 (3): 36–41. Retrieved 19 June 2018.
- "Reducing Urban Heat Islands" (PDF). United States Environmental Protection Agency.
- Shepherd & Woskie. "Controlling Dust from Concrete Saw Cutting" (PDF). Journal of Occupational and Environmental Hygiene. Archived (PDF) from the original on 8 April 2014. Retrieved 14 June 2013.
- General Chipping. "How Does Concrete Recycling Work?", General Chipping. Retrieved on 5 November 2018.
- Occupational Safety and Health Administration. "OSHA’s Respirable Crystalline Silica Standard for General Industry and Maritime", Occupational Safety and Health Administration. Retrieved on 5 November 2018.
- General Chipping. "How Often Should I Plan Concrete Removal for My Drums and Central Mixers?", General Chipping. Retrieved on 5 November 2018.
- "Itaipu Web-site". 2 January 2012. Archived from the original on 9 February 2012. Retrieved 2 January 2012.
- China’s Three Gorges Dam By The Numbers Archived 29 March 2017 at the Wayback Machine. Probeinternational.org. Retrieved on 2017-03-28.
- "Concrete Pouring of Three Gorges Project Sets World Record". People’s Daily. 4 January 2001. Archived from the original on 27 May 2010. Retrieved 24 August 2009.
- "Concrete Pumping to 715 m Vertical – A New World Record Parbati Hydroelectric Project Inclined Pressure Shaft Himachal Pradesh – A case Study". The Masterbuilder. Archived from the original on 21 July 2011. Retrieved 21 October 2010.
- "SCHWING Stetter Launches New Truck mounted Concrete Pump S-36". NBM&CW (New Building Materials and Construction World). October 2009. Archived from the original on 14 July 2011. Retrieved 21 October 2010.
- "Concrete Supplier for Landmark Tower". Archived from the original on 15 May 2013.
- "The world record Concrete Supplier for Landmark Tower Unibeton Ready Mix". Archived from the original on 24 November 2012.
- Al Habtoor Engineering Archived 8 March 2011 at the Wayback Machine – Abu Dhabi – Landmark Tower has a record-breaking pour – September/October 2007, Page 7.
- National Geographic Channel International / Caroline Anstey (2005), Megastructures: Petronas Twin Towers
- "Continuous cast: Exxcel Contract Management oversees record concrete pour". US Concrete Products. 1 March 1998. Archived from the original on 26 May 2010. Retrieved 25 August 2009.
- Exxcel Project Management – Design Build, General Contractors Archived 28 August 2009 at the Wayback Machine. Exxcel.com. Retrieved on 2013-02-19.
- Contractors Prepare to Set Gates to Close New Orleans Storm Surge Barrier Archived 13 January 2013 at the Wayback Machine 12 May 2011
|Wikimedia Commons has media related to Concrete.|
- Chemistry of Concrete at The Periodic Table of Videos (University of Nottingham)
- . . 1914.
- Why Roman concrete still stands strong while modern version decays